 Open Access
 Total Downloads : 11
 Authors : Dr. Prema Kumar W P , Dr. Prathap Kumar M T , Mr. Prasad V
 Paper ID : IJERTV8IS060128
 Volume & Issue : Volume 08, Issue 06 (June 2019)
 Published (First Online): 04062019
 ISSN (Online) : 22780181
 Publisher Name : IJERT
 License: This work is licensed under a Creative Commons Attribution 4.0 International License
Comparative Study on Shear Strength of Steel Fibre reinforced SelfCompacting and Normal Cement Concrete of Grades M30 and M60
Mr. Prasad V Structural Engineer, Bengaluru, India 560 098 
Dr. Prema Kumar W P Professor, School of Civil Engineering, Reva University, Bengaluru, India 560 64 
Dr. Prathap Kumar M T Professor and Head, Department of Civil Engineering, R N S Institute of Technology, Bengaluru, India 560 098 
Abstract Today, selfcompacting concrete (SCC) is the most popular form of concrete that is being delivered by readymix plants (RMC) in India. The construction industry, at present, is using SCC for all major works. There are some areas of construction where normal cement concrete (NCC) is also being used. The main purpose of the present work is to have a comparative idea of the shear strength (using pushoff specimen) of SCC and NCC of grade M30 (representative of normal strength concrete) and M60 (representative of high strength concrete). In the present work, the cube compressive strength and the shear strength (using pushoff specimen) are determined for M30 and M60 grades of selfcompacting concrete and 0.0, 0.5, 1.0 and 1.5 percentages of crimped steel fibres with an aspect ratio of 60. It is observed that the increase in 14 and 28 days compressive strength with fibre percentage is each maximum at 1% of steel fibres for SCC of M30 and M60 grades. The increase in 14 and 28 days shear strength with fibre percentage in the case of SCC of M30 and M60 grades is each observed to be maximum at 1% of steel fibres also. Existing literature reveals that the 14 and 28 days shear strengths increase monotonically as the fibre percentage increases up to 1.5% for both M30 and M60 grades of NCC. For SCC of M30 grade and a given percentage of steel fibres, the shear strength at 14 and 28 days is smaller than that of the corresponding NCC. For SCC of M60 grade and a given percentage of steel fibres, the shear strength at 14 days is greater than that of the corresponding NCC for fibre % up to 0.5. For SCC of M60 grade and a given percentage of steel fibres, the shear strength at 28 days is greater than that of the corresponding NCC for fibre % up to 1.0. Equations for the 28 days shear strength of selfcompacting concrete of grades M30 and M60 as a function of fibre percentage have been developed.
Keywords: Selfcompacting concrete (SCC), Normal cement concrete (NCC), Crimped type steel fibres, Compressive strength, Pushoff specimen, Shear strength.
1.0 INTRODUCTION
Selfcompacting concrete (SCC) was introduced in 1986 in Japan by Hajime Okamura. At present it is the most widely used form of concrete in civil engineering structures. Shear strength of concrete is defined as the ability of concrete to resist forces tangential to the internal planes which are subjected to shear forces or sliding. Many structural members in practice are subjected to shearing forces (direct and indirect). The shear strength of fibrereinforced concrete in flexural members depends on grade of concrete, percentage of steel fibres and percentage of tension steel
provided. In the present experimental work crimped steel fibres are used in the SCC. Shear strength of SCC is determined by using pushoff specimen. The loading on the specimen consists of axial compressive forces (P) applied to the specimen as shown in Fig.1.
Fig.1: Pushoff Specimen and Loading
Vast literature exists on fibre reinforced normal cement concrete as well as on selfcompacting concrete and a very brief review is presented here. Dr.Muhaned A, Shallaland Sallal R, Alowaisy(2008)1 studied the influence of steel fibres on shear transfer strength of concrete by performing pushoff tests. Steel fibres were included along with stirrups crossing the shear plane. 0.0%, 0.5%, 1.0% of steel fibres were used. The results indicated that the use of 1.0% of steel fibres can replace part of stirrups without compromising on shear strength and ductility. J. Jayaprakash et al (2009)2conducted experimental investigation on shear capacity of reinforced concrete precracked pushoff specimens with externally bonded bidirectional carbon fibre reinforced polymer fabrics. In this study the precracked reinforced concrete was externally bonded with carbon fibres. It was observed that the increase in strength varies from 7% to 56% over the unstrengthened reinforced concrete. Rahele Naserianet al (2011)3investigated the interaction of internal steel reinforcement and external fibre reinforced polymer (FRP) composites on the behaviour of shear transfer. 16 non cracked pushoff specimens were tested. It was observed that the effectiveness of FRP strips in unreinforced specimens is significant compared to steel reinforced ones. The shear transfer capacity in strengthened specimens increased from
3% to 38% compared to plain specimens. Constantinescu Horia and Magureanu Cornmelia (2011)4 have used the push off tests to determine the influence of transverse reinforcement on the shear behaviour of high performance concrete with a compressive strength of 100MPa. It was noticed that the contribution of high performance concrete in resisting shear forces is significantly greater than what is currently being considered in structural design. K.C. Denesh (2014)5determined the workability and strength of self compacting concrete of M30 and M40 grades. Crimped steel fibres having an aspect ratio of 80 were used. 0.25%, 0.5%, 0.75% and 1% steel fibres were used. It was found from the results that 1% of fibre gives maximum compressive strength. It was also observed that the flexural strength of concrete increases with the addition of steel fibres to selfcompacting concrete. Javier Echegaray Oviedo et al (2015)6 conducted upgraded PUSHOFF tests to study the mechanism of shear transfer in FRC elements. Pushoff test has been upgraded to control the precracking and in the pushoff stages. Harish Kumar N.R et al (2015)7evaluated inplane shear strength of SCC using inclined plane pushoff specimen. The shear plane inclination was varied (00, 110, 220, and 310). Both plain SCC and reinforced SCC specimens were tested at all the aforesaid inclinations. It was observed that the shear strength increased with the inclination both in plain and reinforced SCC.
The construction industry in India, at present, is using self compacting concrete for all major works. There are some areas of construction where the normal conventional concrete is also being used. In the present work two grades of concrete have been selected viz., M30 (representative of normal strength concrete) and M60 (representative of high strength concrete). The compressive strength (using standard cube specimens) and the shear strength (using push off specimens) are determined for M30 and M60 grades of SCC and 0.0, 0.5, 1.0 and 1.5 percentages of crimped steel fibres in the present work. Chandrashekaramurthy et al 8 have determined the compressive and shear strengths in a similar manner for normal cement concrete (NCC) of M30 and M60 grades. The main objective of this work is to get a comparative idea of compressive strength and shear strength (using pushoff specimens) when NCC is replaced by SCC. A comparison is made between the results of the present work and the results obtained by Chandrashekaramurthy et al
8.
tests in accordance with the Bureau of Indian Standards are given in Table 1.
Table 1: Properties of cement used
Sl. No. 
Physical property 
Value 
1 
Secific gravity 
3.13 
2 
Fineness (%) 
1.2 
3 
Standard consistency (%) 
28 
4 
Initial setting time in minutes 
40 
5 
Final setting time in minutes 
193 
Locally available river sand was used as fine aggregate in the present work. Tests were conducted in accordance with BIS on the river sand used in the present work and the results are furnished in Table 2. Specific gravity and fineness modulus were determined as per IS: 238619689 (Part I) and (Part II). The results of sieve analysis obtained are plotted in Fig.2. Clearly, the fine aggregate used in the present work conforms to ZoneII of IS: 383197010.
Fig.2: Sieve Analysis of Fine Aggregates
Table2: Properties of fine aggregate used
Sl. No. 
Physical property 
Value 
1 
Fineness modulus 
3.95 
2 
Specific gravity 
2.67 
3 
Bulk density (kg/m3) (compacted) 
1603.33 
4 
Bulk density (kg/m3) loose 
1473.32 
5 
Water absorption 
2% 

PRESENT EXPERIMENTAL WORK

Scope

To study the variation of 14 and 28 days compressive strength and shear strength (using push off specimen) of M30 and M60 grades of SCC as the percentage of steel fibres increases from 0.0 to 1.5
% in steps of 0.5%.

To develop equations using regression analysis for the 28 days shear strength of M30 and M60 grades of SCC.

To compare the results of the present work with that of Chandrashekaramurthy et al8.


Materials used
The properties of the 53 grade ordinary Portland cement used in the present work as determined by conducting relevant
Locally available 20mm down size crushed stone aggregates were used in the present work. The properties determined by laboratory testing in accordance with IS: 238619689 are given in Table 3.
Table 3: Properties of coarse aggregate used
Sl No. 
Property 
Result 
1 
Fineness modulus 
4.47 
2 
Specific gravity 
2.79 
3 
Water absorption (%) 
0.44 
4 
Bulk density (kg/m3) Compacted 
1631.65 
5 
Bulk density (kg/m3) Loose 
1425.50 
Master Glenium SKY 8233 superplasticizer was used in the present work to improve the flowability of concrete. First,
the aggregates and cement were mixed with water and later the superplasticizer was added. It is not advisable to add the superplasticizer to dry mix. The new generation Master Glenium is based on modified chains of polycarboxlic ether and it is primarily developed in concrete industry. Potable drinking water supplied by Bengaluru Water Supply and Sewerage Board is used and it meets all the requirements of IS: 302511. The crimped steel fibres used are shown in Fig.3.
Fig.3: Crimped steel fibres
Its properties as furnished by the manufacturer are given in Table 4.
Table 7: Dosage of superplasticizer
% of fibre 
M30 
M60 
0% 
0.60% 
0.80% 
0.50% 
0.60% 
0.85% 
1.00% 
0.70% 
1.00% 
1.50% 
0.85% 
1.25% 
2.4 Workability Tests for SCC
The results of the workability tests conducted on M30 and M60 grades of SCC are given in Tables 8 and 9 respectively. Perusal of these tables clearly reveals that the said M30 and M60 concretes have passed all the required tests for being considered as selfcompacting.
% of fibre 
0 
0.5 
1 
1.5 
Slump Flow Test (mm) 
690 
660 
670 
650 
T50cm Slump Flow (seconds) 
3 
4 
4 
4 
VFunnel Test (seconds) 
10 
10 
9 
9 
VFunnel at T5 (seconds) 
11 
12 
12 
11 
LBox Test (p/p ) 
0.95 
0.95 
0.92 
0.93 
% of fibre 
0 
0.5 
1 
1.5 
Slump Flow Test (mm) 
690 
660 
670 
650 
T50cm Slump Flow (seconds) 
3 
4 
4 
4 
VFunnel Test (seconds) 
10 
10 
9 
9 
VFunnel at T5 (seconds) 
11 
12 
12 
11 
LBox Test (p/p ) 
0.95 
0.95 
0.92 
0.93 
Table 8: Properties of M30 selfcompacting concrete
Table 4: Properties of crimped steel fibres
Sl. No. 
Property 
Value 
1 
Fibre type 
Crimped type fiber 
2 
Length 
30mm 
3 
Diameter 
0.5mm 
4 
Density 
7850 kg/m3 
5 
Tensile strength 
940MPa 
6 
Aspect ratio 
60 
2.3 Mix design
Nan Su method12 is used for the mix design of M30 and M60 grades of SCC in the present work. The mix proportion arrived at for M30 grade of SCC is given in Table 5.
Table 5: Mix proportion for M30 grade of SCC
Cement 
400 kg/m3 
Fine aggregate 
891.35 kg/m3 
Coarse aggregate 
705.625 kg/m3 
Water 
168 kg/m3 
The mix proportion arrived at for M60 grade of SCC is given
in Table 6.
Table 6: Mix proportion for M60 grade of SCC
cement 
545.45 kg/m3 
fine aggregate 
972.395 kg/m3 
coarse aggregate 
769.97 kg/m3 
water 
163.63 kg/m3 
To enhance the workability and make it selfcompacting, superplasticizer, namely, Master Glennium is used in the present work. The dosages of superplasticizer used for M30 and M60 grades of concrete for various percentages of steel fibres are given in Table 7.
Table 9: Properties of M60 selfcompacting concrete
% of fibre 
0 
0.5 
1 
1.5 
Slump Flow Test (mm) 
683 
665 
650 
650 
T50cm Slump Flow (seconds) 
3 
4 
4 
4 
VFunnel Test (seconds) 
9 
8 
9 
9 
VFunnel at T5 (seconds) 
12 
12 
12 
13 
LBox Test (p/p ) 
0.95 
0.95 
0.9 
0.93 

Methodology
Compressive and shear strength tests (using pushoff specimens) were conducted at 14 days and 28 days of curing. Two identical specimens for each percentage of steel fibres and each concrete grade were cast and tested at 14 days. The average of the two values was adopted at 14 days. Three identical specimens for each percentage of steel fibres and each concrete grade were cast and tested at 28 days. The average of the three values was adopted at 28 days. The cubes and pushoff shear strength specimens cast in the present investigation are shown in Fig.4. These specimens were cast following the standard procedure. In the case of pushoff shear strength specimens the wooden piece provided in the groove was removed as shown in Fig.4.
Fig.4: Cubes and pushoff shear strength specimens
2000 kN compression testing machine was used for the experiments. 150 mm x 150 mm x 150 mm size cubes were used for determining the compressive strength. The cube test was conducted as per IS 516: 195913. The compressive load was applied at a rate of 140 kg/cm2/minute. The load at failure for each specimen was noted and the compressive strength computed as usual. The size of pushoff shear strength specimen used was 230 mm x 150 mm x 150 mm. Two wooden planks each of size 160 x 160 x 25 mm were placed at top and bottom to ensure uniform distribution of load over the surface. The load was applied at a rate of 140 kg/cm2/minute. The load at which the specimen fails for each specimen was noted. The shear strength of each specimen was computed using
Shear strength = where shear area = 150 mm x 100 mm
The failed pushoff specimen is shown in Fig.5.
Fig.5: Failed pushoff specimen

Compressive strength test results and discussion

Compressive strength of M30 grade SCC
The results of the compression tests conducted on SCC cubes made of M30 grade concrete at 14 and 28 days are presented in Table 10.
Table 10: Compressive strength results of SCC of M30 grade
%
of steel fibres
Compressive Strength in N/mm2
% Increase in Compressive Strength over that
of the Control Specimen
14
days
28
days
14 days
28 days
0.0 (control specimen)
34.6
36.72
–
–
0.5
36.48
41.59
5.43
13.26
1.0
40.5
45.6
17.05
24.18
1.5
38.47
41.85
11.18
13.97
From Table 10, the following are observed:

The strength developed at 14 days is more than 85% of the 28 day strength for all percentages of steel fibres.

The percentage of increase in the compressive strength of fibrereinforced SCC (both at 14 days and 28 days) over that of unreinforced SCC increases as the fibre percentage increases up to 1% and later decreases.

The increase in 14 and 28 days compressive strength is maximum at 1% of steel fibres.


Compressive strength of M60 grade of SCC
The results of the compression tests conducted on SCC cubes made of M60 grade concrete at 14 and 28 days are presented in Table 11.
Table 11: Compressive strength results of SCC of grade M60
% of steel fibres
Compressive Strength in N/mm2
% Change in Compressive Strength over that
of the Control Specimen
14 days
28 days
14 days
28 days
0 .0 (control specimen)
57.26
64.63
–
–
0.5
59.48
67.4
3.88
(increase)
4.29
(increase)
1.0
59.8
69.4
4.44
(increase)
7.38
(increase)
1.5
42.6
55.36
25.60
(decrease)
14.34
(decrease)
From Table 11, the following are observed:

The strength developed at 14 days is more than 85% of the 28 day strength for all percentages of steel fibres up to 1.0.

The percentage of increase in the compressive strength of fibrereinforced SCC (both at 14 days and 28 days) over that of unreinforced SCC increases as the fibre percentage increases up to 1% and later decreases.

The increase in 14 and 28 days compressive strength is maximum at 1% of steel fibres.



Shear strength test (using pushoff specimen) results and discussion

Shear strength of M30 grade of SCC
The results of the shear strength tests conducted using push off specimens made of SCC M30 grade concrete at 14 and 28 days are presented in Table 12.
Table 12: Shear strength results of SCC of grade M30
% of steel fibres
Shear strength in N/mm2
% Increase in shear
strength over that of the control specimen
14 days
28
days
14 days
28
days
0.0 (control specimen)
5.24
6.47
0.00
0.00
0.5
7.12
8.173
35.88
26.32
1.0
7.82
8.38
49.24
29.52
1.5
6.863
7.102
30.97
9.77
From Table 12, the following are observed:

The strength developed at 14 days is about 80 to 95
% of the 28 days strength.

The percentage of increase in the shear strength of fibrereinforced SCC (both at 14 days and 28 days) over that of unreinforced SCC increases as the fibre percentage increases up to 1% and later decreases.

The increase in 14 and 28 days shear strength is maximum at 1% of steel fibres.


Shear strength of M60 grade of SCC
The results of the shear strength tests conducted using push off specimens on SCC cubes made of M60 grade concrete at 14 and 28 days are presented in Table 13.
Table 13: Shear strength results of SCC of grade M60
% of steel fibres
Shear strength in N/mm2
% Increase in shear strength over that
of the control specimen
14 days
28 days
14 days
28 days
0.0
(control specimen)
6.49
6.98
0.00
0.00
0.5
6.76
7.95
4.16
13.90
1.0
7.19
9.75
10.79
39.68
1.5
7.14
8.28
10.02
18.62
From Table 13, the following are observed:

The strength developed at 14 days is about 75 to 90
% of the 28 days strength.

The percentage of increase in the shear strength of fibrereinforced SCC (both at 14 days and 28 days) over that of unreinforced SCC increases as the fibre percentage increases up to 1% and later decreases.

The increase in 14 and 28 days shear strength is maximum at 1% of steel fibres.


Change of 14 days shear strength of SCC with grade for different % of fibres
The changes in 14 days shear strength of SCC of grades M30 and M60 for different percentages fibers are given in Table 14.
Table 14: 14 days shear strength of M30 and M60 grade SCC for different % fibers
% of steel fibres
M30
(N/mm2)
M60
(N/mm2)
% of change in shear strength
0.00
5.24
6.49
19.26
(increase)
0.50
7.12
6.76
5.33
(decrease)
1.00
7.82
7.19
8.76
(decrease)
1.50
6.86
7.14
3.88
(increase)
From Table 14, it is noticed that the 14 days shear strength decreases as the grade of concrete changes from M30 to M60
for 0.5 and 1.0% of steel fibres, the decrease being not much. Beyond 1.0% there is an increase which is also insignificant. Thus we can say that the increase or decrease in the 14 days shear strength is negligible when the grade of concrete is changed from M30 to M60.

Change of 28 days shear strength of SCC with grade for different % of fibres

The changes in 28 days shear strength of SCC of grades M30 and M60 for different percentages of fibers are given in Table 15.
Table 15: 28 days of shear strength of M30 and M60 grades of SCC for different % of fibers
% of steel fibres 
M30 (N/mm2) 
M60 (N/mm2) 
% of change in shear strength 
0.00 
6.47 
6.98 
7.31 (increase) 
0.50 
8.173 
7.95 
2.81 (decrease) 
1.00 
8.38 
9.75 
14.05 (increase) 
1.50 
7.102 
8.28 
14.23 (increase) 
From Table 15, we can conclude that the increase or decrease in the 28 days shear strength is not very significant when the grade of concrete is changed from M30 to M60.
2.8 Equations for 28 days shear strength of SCC of grades M30 and M60
Equations for the 28 days shear strength of selfcompacting concrete of grades M30 and M60 have been developed at by fitting the best quadratic curve to the points obtained in this experimental work. They are given in Table 16:
Table 16: Equations for the 28 days shear strength (using pushoff specimen)
Grade of SCC 
Equation for 28 days shear strength 
M30 
= 2.981 p2 + 4.8921 p + 6.4705 
M60 
= 2.44 p2 + 4.8 p + 6.775 
Where = shear strength at 28 days in MPa and p = percentage of crimped steel fibres

COMPARISON OF TEST RESULTS ON SCC AND NCC OF GRADES M30 AND M60

General
Chandrashekaramurthy et al have carried out similar experimental studies on NCC (normal cement concrete) of grades M30 (representative of normal strength concrete) and M60 (representative of high strength concrete). A comparison is made between the results of Chandrashekaramurthy et al and that of the present work.

Compressive strength of NCC & SCC of M30 and M60 grades

14 days compressive strength of NCC and SCC of M30 grade
The 14 days compressive strength of NCC and SCC of M30 grade for different percentages of fibres are given in Table 17.
Table 17: 14 days compressive strength of M30 grades of SCC and NCC (MPa)
(%) of steel Fibres
For M30 SCC
For M30 NCC
% difference in 14 days
compressive strength
0.0
34.6
33.37
3.55 (decrease)
0.5
36.48
34.87
4.41 (decrease)
1.0
40.50
35.25
12.96 (decrease)
1.5
38.47
33.26
13.54 (decrease)
From Table 17, the following are observed:

For the same fibre percentage, the compressive strength at 14 days of SCC is greater than that of NCC, the magnitude depending upon on the fibre percentage.

The 14 days compressive strength of SCC and NCC increases as the fibre percentage increases up to 1.0% and later decreases.


14 days compressive strength of NCC and SCC of M60 grade
The 14 days compressive strength of NCC and SCC of M60 grade for different percentages of fibres are given in Table 18.
Table 18: 14 days compressive strength of M60 grades of SCC and NCC (MPa)
% of steel fibres
For M60 SCC
For M60 NCC
% difference in
14 days compressive strength
0.0
57.26
60.22
5.17
(increase)
0.5
59.48
60.78
2.19
(increase)
1.0
59.8
60.78
1.64
(increase)
1.5
42.6
49.32
15.77
(increase)
From Table 18, the following are observed:

For the same fibre percentage, the compressive strength at 14 days of SCC is smaller than that of NCC, the magnitude depending upon on the fibre percentage.

The 14 days compressive strength of SCC and NCC increases as the fibre percentage increases up to 1.0% and later decreases.


28 days compressive strength of NCC and SCC of M30 grade
The 28 days compressive strength of NCC and SCC of M30 grade for different percentages of fibres are given in Table 19.
Table 19: 28 days compressive strength of M30 grades of SCC and NCC (MPa)
% of steel fibres
For M30 SCC
For M30 NCC
% difference in 28 days compressive strength
0.0
36.72
35.25
4.00 (decrease)
0.5
41.59
38.10
8.39 (decrease)
1.0
45.60
38.78
14.96 (decrease)
1.5
41.85
34.00
18.76 (decrease)
From Table 19, the following are observed:

For the same grade of concrete and fibre percentage, the compressive strength at 28days of SCC is greater than that of NCC, the magnitude depending upon on the fibre percentage.

The 28 days compressive strength of SCC and NCC increases as the fibre percentage increases up to 1.0% and later decreases.


28 days compressive strength of NCC and SCC of M60 grade
The 28 days compressive strength of NCC and SCC of M60 grade for different percentaes of fibres are given in Table 20.
Table 20: 28 days compressive strength of M60 grades of SCC and NCC (MPa)
% of steel fibres
For M60 SCC
For M60 NCC
% difference in 28 days compressive strength
0.0
64.63
67.12
3.85(increase)
0.5
67.4
68.40
1.48(increase)
1.0
69.4
68.20
1.73(decrease)
1.5
55.36
50.85
8.15(decrease)
From Table 20, the following are observed:

For the same fibre percentage, the compressive strength at 28 days of SCC is smaller than that of NCC up to 0.5% fibre percentage.

The 28 days compressive strength of SCC increases as the fibre percentage increases up to 1.0% and later decreases.

The 28 days compressive strength of NCC increases as the fibre percentage increases up to 0.5% and later decreases.



Shear strength of NCC & SCC of M30 and M60 grades

14 days shear strength of NCC and SCC of M30 grade
The 14 days shear strength of NCC and SCC of M30 grade for different percentages of fibres are given in Table 21.
Table 21: 14 days shear strength of M30 grades of SCC and NCC (MPa)
% of steel fibres
For M30 SCC
For M30 NCC
% difference in 14 days shear strength
0.0
5.24
7.66
31.59
(increase)
0.5
7.12
7.83
9.07 (increase)
1.0
7.82
9.17
14.72
(increase)
1.5
6.86
10.67
35.68
(increase)
From Table 21, the following are observed:

For the same fibre percentage, the shear strength at 14 days of SCC is smaller than that of NCC, the magnitude depending upon on the fibre percentage.

The 14 days shear strength of SCC increases as the fibre percentage increases up to 1.0% and later decreases.

The 14 days shear strength of NCC increases monotonically as the fibre percentage increases.


14 days shear strength of NCC and SCC of M60 grade
The 14 days shear strength of NCC and SCC of M60 grade for different percentages of fibres are given in Table 22.
Table 22: 14 days shear strength of M60 grade NCC & SCC (MPa)
% of steel fibres
For M60 SCC
For M60 NCC
% difference 14 days shear strength
0.00
6.49
3.33
94.89
(decrease)
0.50
6.76
6.00
12.67
(decrease)
1.00
7.19
8.50
15.41
(increase)
1.50
7.14
9.33
23.47
(increase)
From Table 22, the following are observed:

For the same fibre percentage, the shear strength at 14 days of M60 grade SCC is greater than that of NCC, upto0.5%.

The 14 days shear strength of SCC increases as the fibre percentage increases up to 1.0% and later decreases.

The 14 days shear strength of NCC increases monotonically as the fibre percentage increases.


28 days shear strength of NCC and SCC of M30 grade
The 28 days shear strength of NCC and SCC of M30 grade for different percentages of fibres are given in Table 23.
(%) of steel Fibres
For M30 SCC
For M30 NCC
% difference in 28 days shear strength
0.00
6.47
8.17
20.81 (increase)
0.50
8.17
9.33
12.40 (increase)
1.00
8.38
10
16.20 (increase)
1.50
7.10
11.17
36.42 (increase)
(%) of steel Fibres
For M30 SCC
For M30 NCC
% difference in 28 days shear strength
0.00
6.47
8.17
20.81 (increase)
0.50
8.17
9.33
12.40 (increase)
1.00
8.38
10
16.20 (increase)
1.50
7.10
11.17
36.42 (increase)
Table 23:28 days shear strength of M30 grade NCC & SCC (MPa)
From Table 23, the following are observed:

For the fibre percentage, the shear strength at 28 days of SCC is smaller than that of NCC, the magnitude depending upon on the fibre percentage.

The 28 days shear strength of SCC increases as the fibre percentage increases up to 1.0% and later decreases.

The 28 days shear strength of NCC increases monotonically as the fibre percentage increases.


28 days shear strength of NCC and SCC of M60 grade
The 28 days shear strength of NCC and SCC of M60 grade for different percentages of fibres are given in Table 24.
Table 24: 28 days shear strength of M60 grade NCC &SCC (MPa)
Fibre (%)
For M60 SCC
For M60 NCC
% difference in 28 days shear strength
0.00
6.98
5.50
26.91 (decrease)
0.50
7.95
6.50
22.31 (decrease)
1.00
9.75
8.50
14.71 (decrease)
1.50
8.28
10.33
19.85 (increase)
From Table 24, the following are observed:

For the same fibre percentage, the shear strength at 28 days of M60 grade SCC is greater than that of NCC up to 1.0%, the magnitude depending upon on the fibre percentage.

The 28 days shear strength of SCC increases as the fibre percentage increases up to 1.0% and later decreases.

The 28 days shear strength of NCC increases monotonically as the fibre percentage increases.


4.0 CONCLUSIONS
The following are the important conclusions made from the present work.

Compressive strength of SCC
The 14 days compressive strength of SCC of M30 and M60 grades is, in general, greater than 85% of the 28 days strength. In the case of SCC of M30 and M60 grades, the increase in 28 days compressive strength with fibre percentage is maximum at 1% of steel fibres.

Shear strength of SCC
The 14 days shear strength of SCC of M30 and M60 grades is, in general, greater than about 80% of the 28 days strength. In the case of SCC of grades M30 and M60, the increase in 28 days shear strength is maximum at 1% of steel fibres.

Change in shear strength with increase in the grade of SCC
As the grade of SCC changes from M30 to M60, the change in the 14 days and 28 days shear strengths is small.

Comparison of SCC with NCC

In respect of compressive strength
For M30 grade and a given fibre percentage, the compressive strength at 14 and 28 days of SCC is
greater than that of NCC, the magnitude depending upon on the fibre percentage. For M60 grade and a given fibre percentage, the compressive strength at 14 days of SCC is smaller than that of NCC, the magnitude depending upon on the fibre percentage. For M60 grade, the compressive strength at 28 days of SCC is smaller than that of NCC up to 0.5% of steel fibres.

In respect of shear strength
In case of SCC of M30 grade and a given fibre percentage, the shear strength at 14 and 28 days is smaller than that of NCC, the magnitude depending upon on the fibre percentage. In case of SCC of M60 grade, the shear strength at 14 days is greater than that of NCC, fibre percentage up to 0.5%. In case of SCC of M60 grade, the shear strength at 28days is greater than that of NCC, fibre percentage up to 1.0%. In case of SCC of M30 and M60 grades, the 14 and 28 days shear strengths are maximum at 1% of steel fibres. In case of NCC of M30 and M60 grades, the 14 and 28 days shear strengths increase monotonically as the fibre percentage increases.
REFERENCES

Dr.Muhaned A. Shallaland Sallal R. Alowaisy, Shear Transfer Strength of Steel Fibre Reinforced Concrete,AlQadisiya Journal for Engineering Sciences, Vol.1 (2008).

J. Jayaprakash, Abdul Aziz Abdul Samad and Ashrabov Anvar Abbasvoch., Experimental Investigation on Shear Capacity of Reinforced Concrete Precracked PushOff Specimens with Externally Bonded BiDirectional Carbon Fibre Reinforced Polymer Fabrics, Modern Applied Science Vol.3 (July 2009).

RaheleNaserian, Abdollah Hosseniand Mohammad Sadegh Marefat., Assessment of Shear Transfer Capacity of Non Cracked Concrete Strengthened with External GFRP Strips, Construction and Building Materials Vol.45 Page 224 232(September 2011).

Constantinescu Horiaand Magureanu Cornmelia., Study of Shear Behaviour of High Performance Concrete using Pushoff Tests, JAES 1 (14) Vol.2 (May 2011).

K.C. Denesh,Experimental Study on Fibre Reinforced Self Compacting Concrete, International Journal Engineering Research & Technology, Vol.3 (September 2014).

Javier EchegarayOviedo, Juan NavarroGregori, Estefania Cuenca and Pedro Serna, Upgrading the Pushoff Test to Study the Mechanisms of Shear Transfer in FRC Elements, International Conference on Fracture Mechanics of Concrete and Concrete Structures (2015).

Harish Kumar N.R, Jagannath L, Dr.Nagaraj K.P and Dr.Prabhakara R., Evaluation of InPlane Shear Strength in SCC using Inclined Plane PushOff Specimen, International Research Journal of Engineering and Technology, Vol.02 (July 2015).

Chandrashekaramurthy et al, Shear Strength, Compressive Strength and Workability Characteristics of Concretes reinforced with Steel Fibres, IJERT, Vol.8, Issue 06, June 2019.

IS: 23861968 (Part I) and (Part III), Methods of Test for Aggregates for Concrete, Bureau of Indian Standards, India.

IS: 3831970,Specification for Coarse and Fine Aggregates from Natural Sources for Concrete, Bureau of Indian Standards, India.

IS: 3025 (Part 18),(Part 24),(Part 32) and (Part 17), Methods of Sampling and Test (Physical and Chemical) for Water and Wastewater, Bureau of Indian Standards, India.

Nan Su, K.C.Hsu, H.W.Chai, A Simple Mix Design Method for SelfCompacting Concrete, Cement and Concrete Research 2001.

IS 516 1959, Method of Tests for Strength of Concrete, Bureau of Indian Standards, India.